**Hall-conductivity sign change and fluctuations in amorphous Nb**

_{x}**Ge**

_{1}_{À}

_{x}**films**

Nobuhito Kokubo, Jan Aarts, and Peter H. Kes

*Kamerlingh Onnes Laboratory, Leiden University, P. O. Box 9504, 2300 RA Leiden, The Netherlands*

共Received 8 December 2000; published 11 June 2001兲

The sign change in the Hall conductivity has been studied in thin amorphous Nb1⫺*x*Ge*x(x*⬇0.3) films. By
changing the film thickness it is shown that the field at which the sign reversal occurs shifts to lower values
共*from above to below the mean-field transition field Hc2*) with increasing film thickness. This effect can be
understood in terms of a competition between a positive-normal and a negative-fluctuation contribution to the
Hall conductivity.

DOI: 10.1103/PhysRevB.64.014507 PACS number共s兲: 74.25.Fy, 74.40.⫹k, 74.80.Bj

**I. INTRODUCTION**

One of the puzzling and intriguing phenomena in type-II
superconductors is the sign change in the Hall effect near the
*mean-field transition at the upper critical field Hc2*. Such a

Hall anomaly has been observed in some conventional

*low-Tc* superconductors, such as, moderately disordered Nb and

V共Ref. 1兲and amorphous MoSi共Refs. 2 and 3兲and MoGe

共Ref. 4兲 *films, as well as most high-Tc* superconductors
共HTSC兲.5 *Hagen et al.*5 pointed out the importance of the
electron mean-free path for the Hall anomaly and concluded
that very clean and very dirty materials do not show Hall
anomalies. However, studies on amorphous dirty
supercon-ductors contradict this conclusion.2–4

Recent phenomenological approaches based on the time-dependent Ginzburg-Landau共TDGL兲equation have qualita-tively explained the sign anomaly.6–8 In these theories, the sign reversal is just a consequence of the difference in sign between the normal共or quasiparticle兲term and the supercon-ducting fluctuation共or vortex flow兲term of the Hall conduc-tivity. Several authors9–12 have derived the sign of the fluc-tuation共vortex flow兲term from the TDGL equation for BCS superconductors. Recent experimental studies13 on HTSC’s have pointed out that the sign predictions of these theories are not correct for HTSC’s, but they should be valid for BCS superconductors.

Even if the sign of the Hall-fluctuation conductivity were
clear, its temperature and field dependence is a matter of
discussion. Recent experimental studies on YBa2Cu3O7⫺␦
films14–16 and single-crystalline Bi2Sr2CaCu2O8_{⫹}␦ and
Bi1.95Sr1.65La0.4CuO6⫹␦共Ref. 17兲have observed that the sign
*change takes place above Hc2*, while other studies have

*claimed that the sign anomaly takes place below Hc2*. In this

*problem, the definition of Hc2*as well as the temperature and

field dependence of the Hall-fluctuation conductivity is very important.

As reported in conventional amorphous films18 as well as
HTSC’s, the longitudinal conductivity in a perpendicular
magnetic field shows a smooth crossover from the
*paracon-ducting regime to flux-flow regime around Hc2*, which is

strikingly different from the picture of the conventional
fluc-tuation theory in which the conductivity due to the direct
fluctuation contributions of the Aslamazov-Larkin共AL兲
*pro-cess diverges at Hc2*.

19

*Thus, it was difficult to define Hc2*

correctly from the fluctuation theory. Recent TDGL

theories,6 however, have successfully explained the smooth
*crossover around H _{c2}*by taking into account the interaction
term of superconducting fluctuations of the AL process
within the Hartree approximation. Later, Ullah and Dorsey

共UD兲 共Ref. 7兲developed this further and proposed a scaling
theory for the longitudinal and Hall conductivities. This
*scal-ing approach is very useful to determine Hc2*correctly and to

describe the field and temperature dependence of the conduc-tivities.

In this paper, we present measurements and analysis of
the longitudinal and Hall resistivities *xx* and *y x* for thin

amorphous 共a-兲 Nb_{1}_{⫺}* _{x}*Ge

_{x}*(x*⬇

*0.3) films (T*⬇3 K) ac-cording to the TDGL theories. We confirm that the smooth

_{c}*crossover in the longitudinal conductivity around Hc2*is well

explained by the UD scaling theory as was found
previously,20 *and determine Hc2*. We then show that for the

thinner films the sign change in the Hall conductivity takes
*place above H _{c2}*. Contrary to results on HTSC’s, we show
that the sign of the Hall conductivity is consistent with the
TDGL theory for BCS superconductors. We discuss the
ori-gin of the sign reversal observed here.

**II. EXPERIMENT**

The films used in this study were deposited by rf
sputter-ing on Si substrates held at room temperature in a system
with a base pressure of 10⫺6 mbar, using 10⫺2 mbar Ar gas
as a sputtering gas. The thicknesses used were 16, 34, 60,
and 163 nm. X-ray diffraction showed the films to be
amor-phous. The average composition for each film was
deter-mined by electron-microprobe analysis. The distribution in
the composition ␦*x is less than 1%. The superconducting*

*mean-field transition temperature in zero field, Tc*, was

de-termined from the temperature dependence of resistivity by
using the AL fluctuation theory.21 From a previous
*system-atic study on a-Nb*_{1}_{⫺}* _{x}*Ge

*films,22*

_{x}*the distribution of T*due to ␦

_{c}*x is estimated to be less than 18 mK (*␦

*T/Tc*ⱗ6

⫻10⫺3*) around x*⫽0.3. Except for the film thickness, these
films have the following identical parameters; the average
*composition x*⬇*0.3, Tc*⬇3 K, the normal-state resistivity

*xx*

*n* _{⬇}_{2.2} _{}_{⍀}_{m,} _{S}_{⬅}_{⫺}_{d(}_{}

0*Hc2)/dT*兩*T _{c}*⬇2 T/K, the

eight voltage and two current contacts. The longitudinal and
Hall resistivities are measured by a conventional dc
four-probe method. The longitudinal component due to the
mis-alignment in the Hall probes was subtracted by reversing the
field direction. The films are immersed in liquid 4He to
ob-tain good thermal contact. The magnetic field is normal to
the film surface. The normal resistivity * _{xx}n* in the
tempera-ture range of 1.5 K⬍

*T*⬍5 K has a small temperature coef-ficient (

*)⫺1*

_{xx}n*d*

*n*⬃⫺10⫺4 K⫺1.

_{xx}/dT**III. RESULT AND DISCUSSION**

In this study,*xx*(⫽*Ex/Jx*) and*y x*(⫽*Ey/Jx*) were

*mea-sured as a function of H (*兩0*H*兩⬉*8 T) at various T. Figures*
1共a兲 and 1共b兲show the field dependence of the longitudinal
*xx*关⬅*xx*/(*xx*

2 _{⫹}_{}

*y x*

2 _{)}_{兴} _{and} _{Hall} _{conductivities} _{}

*xy*
关⬅*y x*/(*xx*

2 _{⫹}_{}

*y x*

2 _{)}_{兴} _{at different T for the 34-nm-thick film}

*with Tc*⫽2.77 K. To reduce the effect of pinning in the

*mixed state, the measuring current density J was selected to*
be 1.4⫻107 A/m2 that is much higher than the depinning
*current density Jc*(⬃105 A/m2), but smaller than the

depair-ing current density (⬃1010 A/m2).

*Far above Tc*, *xx* is field independent while*xy* is

*di-rectly proportional to H, that is, the normal-state Hall effect*
appears. The normal-state Hall conductivity *xy*

*n*

has a
posi-tive sign. Within the Drude model, the normal-state Hall
angle, tan* _{H}n* , is given by

tan* _{H}n*⬅

*/*

_{xy}n*⫽*

_{xx}n*c*, 共1兲

where * _{c}* is the cyclotron frequency and is the elastic
scattering time of electrons. Compared with typical result on
HTSC’s (

*c*⬃10⫺2 at0

*H*⫽1 T), the present films have very small value of

*c*⬃10⫺5at0

*H*⫽1 T, indicating the very small mean-free path to be expected for amorphous metals.

*Near and below T _{c}* one can clearly see that

*changes*

_{xy}*sign at a certain field H**in Fig. 1共b兲. We do not observe any

*second sign change below H**, in contrast to what has been reported for several HTSC’s.23

*Far above H**,

*xy*recovers

*the direct proportionality to H and the normal-state Hall *
ef-fect appears again, indicating that the superconducting
fluc-tuations are completely suppressed by magnetic field. We
therefore can define *xy*

*n*

*below Tc* unambiguously.

*In order to determine Hc2*, we use the UD scaling theory.

According to this theory, the longitudinal conductivity is
composed of the normal 共or quasiparticle兲 term * _{xx}n* and
superconducting-fluctuation共or vortex-flow兲term␦

*xx*, and

expressed as

*xx*⫽*xx*
*n* _{⫹}_{␦}

*xx*. 共2兲

␦*xx* interpolates smoothly from the paraconducting regime

*to flux-flow regime around H _{c2}*and obeys universal scaling

*functions F˜*

_{⫾}

*where F˜*

_{⫹}

*(F˜*

_{⫺}

*) is the scaling function for H*⬎

*Hc2(H*⬍

*Hc2*). These functions depend on the

*dimension-ality governed by the ratio of the film thickness d and the*
length scale for fluctuations of the order parameter near

*Hc2*. For the thickness of the films in this study we can apply

two-dimensional 共2D兲 scaling functions.20 *At each T we*
identify * _{xx}n* with

*xx*taken at a field 共typically 7 T兲where

*xy* depends linearly on field and *xx* is field independent.

␦*xx* is obtained by subtracting *xx*

*n* _{from} _{}

*xx*. Figure 2

shows a typical scaling result. Here, the data are plotted
*above Hc2(T)/3 where the lowest Landau level* 共LLL兲

ap-proximation for the scaling functions is valid.20 One can
clearly see that the scaled longitudinal fluctuation
*conductiv-ity F˜ _{xx}2D*兵⬅␦

*xx*/关

*C*

*xx*

*n*

*(A*_{0}*2Dt/h)*1/2兴其 collapses on two
*uni-versal curves F˜*_{⫾} *as a function of the scaled field x2D*given
*by x2D*⬅⑀*H*/

## 冑

*A*0

*2D*

*th, with* ⑀*H*⫽0关*H*⫺*Hc2(T)*兴*/STc*,

al-though deviations are visible at large 兩*x2D*兩*. Here, t*⫽*T/Tc*

*and h*⫽0*H/STc* are normalized temperature and field,

*re-spectively. C is related to the real part of the relaxation time*
of the order parameter ␥⫽␥1⫹*i*␥2. We take a dirty limit
*value of C*⫽1.447.20The strength of thermal fluctuations for
*2D system, A*_{0}*2D, is given by A*_{0}*2D*⫽4

## 冑

*2Gi*

*GL(0)/d where*

FIG. 1. The field dependence of 共a兲 the longitudinal,共b兲 Hall,
and共c兲*Hall-fluctuation conductivities at different T of 2.08 K (*䊊),
2.20 K (䊐), 2.47 K (䉭), 2.60 K (〫), and 3.71 K (ⵜ) for a
34-nm-thick film. The short and long arrows denote the
*sign-reversal field H** *and the mean-field transition field Hc2*,

*Gi*(⬇5⫻10⫺6) is the Ginzburg number.24 Very close to
*Hc2*, deviations due to the inhomogeneity in the composition

␦*x become apparent. Hence, we do not plot the data in fields*
兩⑀*H*兩⬍(1/2)␦*Tc/Tc*⬇3⫻10⫺3, which roughly corresponds

to 兩*x2D*兩⬍0.2. In such a scaling plot, the unknown
*param-eters are S and Hc2(T). In the temperature range close to Tc*,

*they are connected by the simple relation Hc2(T)*⫽*S(Tc*

⫺*T). We first determine S from the scaling collapse of the*

*data close to Tcand this S value is used to determine Hc2*far

*below T _{c}* in the scaling analysis. Thus, we can

*unambigu-ously determine Hc2*from the scaling collapse of the data.

*Before proceeding to the result of the H _{c2}* line, we

*com-pare the scaling functions F˜*

_{⫾}with those predicted in the UD theory. The UD theory implies that the 2D universal

*func-tions F˜*

_{⫾}

*2D*in the high-field limit are given by

*x2D*⫽*1/F˜2D*⫺*F˜2D*, 共3兲

if the pinning effect in the flux-flow regime is negligible and
the fluctuation conductivity in the paraconducting regime is
dominated by the direct fluctuation contributions of the AL
process. These functions are applicable to the field range
where the LLL is satisfied. The solid lines in Fig. 2共a兲denote
*these universal functions. F˜*_{⫾} *agrees well with F˜*_{⫾}*2D* near

*H _{c2}*(⫺1ⱗ

*x*ⱗ6), while deviations are visible in the large

_{2D}兩*x2D*兩 *regime. In the paraconducting regime, F˜*_{⫹} decreases
*much faster than F˜*_{⫹}*2D* *above x2D*⬇6. Such a rapid decrease
in␦*xxwas also observed far above Hc2*in amorphous thick

films and attributed qualitatively to a phenomenological
short-wavelength cutoff in the fluctuation spectrum.25For the
*other films (d*⫽16 and 60 nm兲 except for the thickest film
*(d*⫽163 nm),26*similar deviation of F˜*_{⫹}begins to appear at

*almost the same value of x2D*⬇6, although the physical
ori-gin of the short-wavelength cutoff is not clear. The definition
of * _{xx}n* does not affect this behavior because the field at
which

*is defined is much larger than the fields of interest.*

_{xx}n*Hereafter, we regard x2D*⫽6 as the phenomenological boundary below which ␦

*is well described by the UD scaling theory, and discuss our data below this boundary.*

_{xx}From the scaling collapse of ␦*xx* *we obtained the Hc2*

line for films with different thicknesses. To compare those
results, we plot the normalized mean-field value of
0*Hc2/STc*(⬅*hc2) against normalized temperature T/Tc*for

*different films in Fig. 3. Good agreement is seen for H _{c2}*of
all films. The solid line represents the mean-field line for the
dirty limit in the Werthamer-Helfand-Hohenberg 共WHH兲
theory, which is given by

ln共*t*兲⫽⌿共1/2兲⫺⌿关1/2⫹共2/2兲*hc2/t*兴, 共4兲

where⌿ is the digamma function.27*The Hc2*line obtained is

well approximated by this relation, giving experimental sup-port for the validity of the UD scaling theory.

Next, we turn to results of the Hall-fluctuation conductiv-ity. In the TDGL theories,7 the Hall conductivity also con-sists of a normal共or quasiparticle兲term and a superconduct-ing fluctuation 共or vortex flow兲term,

*xy*共*H,T*兲⫽*xy*
*n* _{共}

*H,T*兲⫹␦*xy*共*H,T*兲. 共5兲

Hence, we subtract *xy*
*n*

*(H,T) from* *xy(H,T), and plot*

␦*xy(H,T) against H in Fig. 1*共c兲. The plot shows that␦*xy*

*always has a negative sign. Hc2* is denoted by the long

*ar-rows. With decreasing H the magnitude of* ␦* _{xy}* increases

*monotonically and grows as 1/H at low H (*Ⰶ

*Hc2*) 共not

shown兲as the TDGL theories predict.28Thus, the sign
rever-sal of_{xy}*at H** always takes place when␦* _{xy}* and

*are different in sign. Beforehand it is not clear whether or not FIG. 2. The scaled fluctuation conductivity plotted as a function*

_{xy}nof兩*x2D*_{兩} _{at different T of 2.08 K, 2.20 K, 2.47 K, and 2.60 K. The}

*current density J is 2.94*⫻107 A/m2except for the curve at 2.08 K
*where J*⫽1.47⫻107 _{A/m}2_{. The symbols correspond to those in}

Fig. 1. The solid curves represent the 2D universal scaling functions
*F*

*˜*_{⫾}*2D*

*. S is found to be 2.16 from the scaling collapse of the data*
*taken at 2.47 K and 2.60 K close to Tc*⫽*2.77 K. The Hc2*values

for 2.08 K and 2.20 K are determined from the scaling collapse of
*the data using this S value.*

FIG. 3. 0*Hc2/STc* *plotted as a function of T/Tc* for different

films of 16 nm (䊏), 34 nm (䊉), 60 nm (䉱), and 163 nm (⽧) thickness. The solid curve represents the mean-field line in the dirty limit for the WHH theory. The corresponding open symbols show

0*H**/ST*cfor the same films plotted against T/Tc*. The dashed and

dashed-dotted lines represent the phenomenological boundaries

*H** *is above Hc2*, because*xy*
*n*

and␦*xy* depend in different

ways on the electronic structure of the material. As one can
*see in Fig. 3, in the thinnest film H** 共denoted by open
sym-bols兲 *is always above H _{c2}* but below the phenomenological
boundary where scaling analysis starts to fail. It may be

*worth pointing out that H** decreases monotonically with

*rising T and terminates finally at a certain T**

*above Tc0*in

*zero field. With increasing d, H** moves systematically
*closer to H _{c2}* and it finally shifts below 共but very close to兲

*Hc2* for the thickest film, implying that the contribution of

the negative ␦*xy* to positive*xy*
*n*

decreases with increasing

*d. These results support the view that enhancing the *

*super-conducting fluctuations by reducing d leads to an increasing*
negative Hall conductivity working against positive * _{xy}n* ,

*which is responsible for the sign reversal above Hc2*.

We now discuss the field and temperature dependences of
␦*xy*, in comparison with the UD scaling theory. According

to this theory,␦*xx* and␦*xy* have the same field and

tem-perature dependence and their ratio should be independent of

*H and T. Note that* ␦*xy*/␦*xx*⫽⫺␥2/␥1, the ratio of the
imaginary and real part of ␥.7 We did not find scaling of
␦*xy*. A recent study on YBa2Cu3O7⫺␦ films14 has pointed
out that the failure of the scaling of␦* _{xy}*can be attributed to
the additional contributions of the Maki-Thompson 共MT兲
process, which are not taken into account in the UD theory.
However, the MT process cannot explain the present result
because the strong pair-breaking effect in the amorphous
dirty films should lead to a small contribution.25,29 As one

can see in the inset of Fig. 4共a兲, contrary to the UD scaling
theory, ⫺␦*xy*/␦*xx* *at Hc2* increases monotonically with

cooling. Similar temperature dependence of ⫺␦*xy*/␦*xx*

has been reported for amorphous MoSi films.3We conclude
that the main reason for the scaling failure is the temperature
dependence of ␥2/␥1. Further microscopic calculations
based on the BCS theory are required to explain this effect.
The field dependence of ⫺␦*xy*/␦*xx* is shown in Fig.

4共a兲for two current densities. In the field range (⫺1ⱗ*x2D*

ⱗ6) where ␦* _{xx}* follows the UD scaling theory,
⫺␦

*xy*/␦

*xx*

*is independent of J and depends only weakly*

*on x2D*. As one can see in Fig. 4共b兲, however, in the same
field range both conductivities change almost one decade in
*magnitude and their dependences on x2D* look very similar.
Hence, we believe that both␦*xx* and␦*xy* in the

paracon-ducting regime (0⭐*x2D*_{ⱗ}_{6) are dominated by the direct}
fluctuation contributions of the AL process and thus the
con-tributions of the AL process are responsible for the sign
*change of the Hall conductivity above Hc2*.

Finally, we discuss the origin of the sign in*xy*
*n*

and␦*xy*

for our amorphous films. The sign of * _{xy}n* depends on the
sign of the group velocity

*v*关⬅(1/ប)/

*k*兴 of electrons at the Fermi level where

*is the energy and k is the wave*number. Because of the absence of band structure, the amor-phous materials are generally more free-electron-like than their crystalline counterparts. Therefore, the simple amor-phous metals generally have negative

*because of a posi-tive group velocity (*

_{xy}n*v*⬀

*k*⬎0).30 Most of the amorphous transition metals 共TM’s兲, however, have positive

*.31The origin of this positive *

_{xy}n

_{xy}n*has been attributed to the s-d*hybridization interaction in the TM, which leads to a nega-tive group velocity (/

*k*⬍0) at the Fermi level if the Fermi energy

*F*

*lies within the d band.*31–33 The

TM-metalloid-type amorphous superconductors NbGe as well as
MoGe and MoSi belong to amorphous TM’s and have
posi-tive *xy*

*n*

.

In the TDGL theory based on BCS superconductors by
Nishio and Ebisawa,10the sign of␦*xy* is determined by the

electron-hole asymmetry, i.e., by the sign of ⫺*N*

### ⬘

, where*N*

### ⬘

关⬅*dN(*

*)/d*兩

_{⫽}

*F*兴 is the energy derivative of the
den-sity of states 共DOS兲 *N(*) at the Fermi energy. Numerical
calculations of the DOS for, e.g., amorphous Ni imply32that
the total DOS near _{F}*is dominated by the DOS for the d*
band whose energy dependence is characterized by a peak
*near the center of d-band**d* and roughly approximated by a

parabolic energy dependence with negative curvature, i.e.,

*N(*)⬀⫺(⫺*d*)2. Similar energy dependences of the total

DOS have been commonly observed for various amorphous
TM-metalloid alloys by photoemission experiments.34
*Be-cause Nb is a less than half-filled 4d-band metal,* *F* lies

*below the center of the 4d-band* *4d. Thus, a-NbGe films*
*have positive N*

### ⬘

*. The same argument holds for a-MoGe and*

*MoSi, since Mo is also a less than half-filled 4d-band metal.*Thus, sgn(␦

*)⫽sgn(⫺*

_{xy}*N*

### ⬘

)⬍*0 in both a-NbGe, a-MoGe,*

*and a-MoSi films.*2–4These findings give experimental sup-port for the prediction of the sign of ␦

*in the TDGL theory for BCS superconductors.*

_{xy}FIG. 4. 共a兲 The ratio of the fluctuation conductivities,

⫺␦*xy*/␦*xx, plotted as a function of x2D* *at T*⫽2.08 K for the

*34-nm-thick film with different J of 1.4 kA/cm*2 _{(}_{䊊}_{) and}

4.4 kA/cm2 (䊐).共b兲The corresponding longitudinal (䊊,䊐) and
Hall fluctuation conductivities (䊉,䊏) are also plotted as a function
*of x2D* *with different J. Inset in*共a兲*shows the T/Tc*dependence of
␥2/␥1(⫽⫺␦*xy*/␦*xx) at Hc2*with different thickness of 16 nm

**IV. SUMMARY**

In summary, we have measured the longitudinal and Hall resistivities for thin films of the dirty superconductor

*a-Nb*1_{⫺}*x*Ge*x(x*⬇*0.3) near Hc2*. We confirm that␦*xx*obeys

the 2D scaling functions of the UD fluctuation theory. We
*find a good agreement of the obtained Hc2* line with the

WHH theory, supporting the scaling procedure. The failure
of the scaling collapse of␦*xy* is attributed to the

tempera-ture dependence of␥2/␥1. The Hall conductivity*xy*in

*thin-ner films shows a sign change at a certain H**that is above

*Hc2* but in the regime where *xx* follows the UD theory.

*With increasing film thickness, H***moves closer to H _{c2}*and
it finally shifts below共but close to兲

*Hc2*for the thickest film.

The negative contribution of the superconducting
fluctua-tions of the AL process working against positive * _{xy}n* is

*re-sponsible for the sign change above Hc2*. The negative sign

of ␦*xy* in the present films is consistent with the

electron-hole asymmetry in the framework of the TDGL theory for BCS superconductors.

**ACKNOWLEDGMENTS**

We are very grateful to R. Ikeda for useful comments and sending us his manuscripts. We would like to thank Y. Mat-suda for giving us a copy of his unpublished work. We ac-knowledge the experimental assistance of R. Besseling, M.B.S. Hesselberth, G.L.E. van Vliet, R.W.A. Hendrikx, and T.J. Gortenmulder. This work was part of the research pro-gram of the ‘‘Stichting voor Fundamenteel Onderzoek der Materie’’ 共FOM兲, which is financially supported by NWO. One of the authors共N.K.兲was financially supported by JSPS.

1_{K. Noto, S. Shinzawa, and Y. Muto, Solid State Commun. 18,}

1081共1976兲.

2_{A.W. Smith, T.W. Clinton, C.C. Tsuei, and C.J. Lobb, Phys. Rev.}

**B 49, 12 927**共1994兲.

3_{A.W. Smith, T.W. Clinton, W. Liu, C.C. Tsuei, A. Pique, Q. Li,}

**and C.J. Lobb, Phys. Rev. B 56, 2944**共1997兲.

4** _{J.M. Graybeal, J. Luo, and W.R. White, Phys. Rev. B 49, 12 923}**
共1994兲.

5_{S.J. Hagen, A.W. Smith, M. Rajeswari, J.L. Peng, Z.Y. Li, R.L.}

Greene, S.N. Mao, X.X. Xi, S. Bhattacharya, Qi Li, C.J. Lobb,
**Phys. Rev. B 47, 1064**共1993兲.

6** _{R. Ikeda, T. Ohmi, and T. Tsuneto, J. Phys. Soc. Jpn. 58, 1377}**
共1989兲

**; 59, 1397**共1990兲

**; 60, 1051**共1991兲.

7_{S. Ullah and A.T. Dorsey, Phys. Rev. B 44, 262}_{共}_{1991}_{兲}_{.}
8

**N.V. Kopnin and A.V. Lopatin, Phys. Rev. B 51, 15 291**共1995兲.
9_{H. Fukuyama, H. Ebisawa, and T. Tsuzuki, Prog. Theor. Phys.}

**46, 1028**共1971兲.

10_{T. Nishio and H. Ebisawa, Physica C 290, 43}_{共}_{1997}_{兲}_{.}

11** _{A.G. Arnov and A.B. Rapoport, Mod. Phys. Lett. B 6, 1083}**
共1992兲; A.G. Arnov, S. Hikami, and A.L. Larkin, Phys. Rev. B

**51, 3880**共1995兲.

12_{A. van Otterlo, M. Feigel’man, V. Geshkenbein, and G. Blatter,}

**Phys. Rev. Lett. 75, 3736**共1995兲; M.V. Feigel’man, V.B.
Gesh-kenbein, A.I. Larkin, and V.M. Vinokur, Pis’ma Zh. E´ ksp. Teor.
**Fiz. 62, 811**共1995兲 关**JETP Lett. 62, 834**共1995兲兴; D.I. Khomskii
**and A. Freimuth, Phys. Rev. Lett. 75, 1384**共1995兲.

13_{T. Nagaoka, Y. Matsuda, H. Obara, A. Sawa, T. Terashima, I.}

**Chong, M. Takano, and M. Suzuki, Phys. Rev. Lett. 80, 3594**
共1998兲.

14_{W. Liu, T.W. Clinton, A.W. Smith, and C.J. Lobb, Phys. Rev. B}

**55, 11 802**共1997兲.

15_{A.V. Samoilov, Phys. Rev. B 49, 1246}_{共}_{1994}_{兲}_{.}

16_{W. Lang, G. Heine, P. Schwab, X. Z. Wang, and D. Ba¨uerle,}

**Phys. Rev. B 49, 4209**共1994兲.

17_{R. Jin and H.R. Ott, Phys. Rev. B 53, 9406}_{共}_{1996}_{兲}_{.}
18_{P. Berghuis and P.H. Kes, Phys. Rev. B 47, 262}_{共}_{1992}_{兲}_{.}
19_{For example, K. Maki, J. Low Temp. Phys. 1, 513}_{共}_{1969}_{兲}_{.}
20_{M.H. Theunissen and P.H. Kes, Phys. Rev. B 55, 15 183}_{共}_{1997}_{兲}_{.}

21_{L.G. Aslamazov and A.I. Larkin, Phys. Lett. 26A, 238}_{共}_{1968}_{兲}_{.}
22

R. Wo¨rdenweber, A. Pruymboom, and P.H. Kes, J. Low Temp.
**Phys. 70, 253**共1987兲.

23_{For example, W.N. Kang, B.W. Kang, Q.Y. Chen, J.Z. Wu, S.H.}

Yun, A. Gapud, J.Z. Qu, W.K. Chu, D.K. Christen, R. Kerchner,
**and S.W. Chu, Phys. Rev. B 59, 9031**共1999兲.

24_{C.J. Lobb, Phys. Rev. B 36, 3930}_{共}_{1987}_{兲}_{.}

25_{W.L. Johnson, C.C. Tsuei, and P. Chaudhari, Phys. Rev. B 17,}

2884共1978兲.

26_{The deviations from the 2D scaling functions observed for the}

thickest film are different from those observed for the thinner
*films. With increasing x2D* *F˜*_{⫹} for the thickest film exhibits
*much slower decrease than F˜*_{⫹}*2D*. This stems from the
dimen-sional crossover, although the 3D limit analysis is not fully valid
yet共Ref. 20兲. We believe that for the thickest film the 2D scaling
*analysis is still valid in a narrow field range near Hc2. Hc2*
obtained from the 2D scaling analysis is plotted in Fig. 3.
27_{N. Werthamer, E. Helfand, and P.C. Hohenberg, Phys. Rev. 147,}

295共1966兲.

28_{A.T. Dorsey, Phys. Rev. B 46, 8376}_{共}_{1992}_{兲}_{; R.T. Troy and A.T.}

* Dorsey, ibid. 47, 2715*共1993兲.

29** _{W.F. Skocpol and M. Tinkham, Rep. Prog. Phys. 38, 1049}**
共1975兲.

30_{U. Mizutani, Prog. Mater. Sci. 28, 97}_{共}_{1983}_{兲}_{.}

31_{B.L. Gallagher, D. Greig, M. A. Howson, and A.A.M. Croxon, J.}

**Phys. F: Met. Phys. 13, 119**共1983兲.

32_{G.F. Weir, M.A. Howson, B.L. Gallagher, and G.J. Morgan, }

**Phi-los. Mag. B 47, 163** 共1983兲*; G.J. Morgan and G.F. Weir, ibid.*
**47, 177**共1983兲.

33** _{G.F. Weir and G.J. Morgan, J. Phys. F: Met. Phys. 11, 1833}**
共1981兲.

34_{W.L. Jonson, J. Appl. Phys. 50, 1557}_{共}_{1979}_{兲}_{; B. Schro¨der, W.}